# Micromechanical Modeling of Fatigue Crack Nucleation around Non-Metallic Inclusions in Martensitic High-Strength Steels

^{1}

^{2}

^{*}

## Abstract

**:**

## 1. Introduction

## 2. Material and Experimental Investigations

#### 2.1. Martensitic Microstructure

#### 2.2. Failure-Relevant Non-Metallic Inclusions

## 3. Modeling Methodology and Constitutive Model

#### 3.1. Modeling Statistical Volume Elements

#### 3.1.1. Modeling Martensitic Statistical Volume Elements without Defects

#### 3.1.2. Modeling Martensitic Statistical Volume Elements with Defects

#### 3.2. Local Crystal Plasticity Model

#### 3.2.1. Constitutive Equations

#### 3.2.2. Calibration of the Crystal Plasticity Model

#### 3.3. Simulation Methodology for Residual Stress Development

#### 3.4. Fatigue Indicator Parameters and Fatigue Crack Nucleation Model

#### 3.5. Strategy of the Numerical Design of Experiment

## 4. Results and Discussion

#### 4.1. Influence of Microstructural Variability

#### 4.2. Effect of Residual Stresses

#### 4.3. Influence of Interface Properties on Fatigue Response

#### 4.4. Influence of Defect Size

#### 4.5. Influence of Aspect Ratio of Voids

#### 4.6. Influence of Manganese Sulfide Aspect Ratio and Orientation

#### 4.7. Fatigue Crack Initiation Lifetime Results

## 5. Conclusions

- Residual stresses around oxidic inclusions
- Microstructural variability around defects
- Varying interface properties between non-metallic inclusions and the surrounding matrix
- Defect size
- Defect shape
- Alignment of manganese sulfides to loading axis

- The consideration of the residual stresses around oxidic inclusions due to previous heat treatments result in an increased fatigue crack nucleation potential, in particular for fatigue loading levels close to the elastic regime.
- The local fatigue crack nucleation responses around defects and inclusions depend strongly on the defect size, defect shape, martensitic block size and the crystallographic properties at the hot spot. Therefore, multiple martensitic microstructural realizations were considered in the numerical study to create a certain kind of statistical basis.
- In the present study, voids with increasing aspect ratios represent the most severe defects under fully reversed strain-controlled loading conditions. In particular, for loading levels within the elastic regime, the different inclusion–matrix interface conditions influence the fatigue crack nucleation lives substantially.
- The micromechanical investigations of the manganese sulfide fatigue crack nucleation behavior exhibit an influence of the aspect ratio (size of manganese sulfide) as well as a significant influence of the alignment of the manganese sulfide to the loading axis. These results correlate qualitatively well with the corresponding experimentally observed fracture behavior.

## Author Contributions

## Funding

## Conflicts of Interest

## References

- Lewis, A.M.; Kelly, J.C.; Keoleian, G.A. Vehicle lightweighting vs. electrification: Life cycle energy and GHG emissions results for diverse powertrain vehicles. Appl. Energy
**2014**, 126, 13–20. [Google Scholar] [CrossRef] - Tervo, H.; Kaijalainen, A.; Pikkarainen, T.; Mehtonen, S.; Porter, D. Effect of impurity level and inclusions on the ductility and toughness of an ultra-high-strength steel. Mater. Sci. Eng. A
**2017**, 697, 184–193. [Google Scholar] [CrossRef] - Murakami, Y. Metal Fatigue: Effects of Small Defects and Nonmetallic Inclusions, 1st ed.; Elsevier: Oxford, UK, 2002. [Google Scholar]
- Yang, Z.; Zhang, J.; Li, S.; Li, G.; Wang, Q.; Hui, W.; Weng, Y. On the critical inclusion size of high strength steels under ultra-high cycle fatigue. Mater. Sci. Eng. A
**2006**, 427, 167–174. [Google Scholar] [CrossRef] - Klösch, G.; Huemer, K.; Frank, G. Nichtmetallische Einschlüsse in Langprodukten: Entstehung, Bestimmung, Auswirkungen—Ein Überblick. BHM Berg-Und Hüttenmännische Monatshefte
**2009**, 154, 27–32. [Google Scholar] [CrossRef] - Krewerth, D.; Lippmann, T.; Weidner, A.; Biermann, H. Influence of non-metallic inclusions on fatigue life in the very high cycle fatigue regime. Int. J. Fatigue
**2016**, 84, 40–52. [Google Scholar] [CrossRef] - Juvonen, P. Effects of Non-Metallic Inclusions on Fatigue Properties of Calcium Treated Steels. Ph.D. Thesis, Helsinki University of Technology, Espoo, Finland, 2004. [Google Scholar]
- Tanaka, K.; Mura, T. A theory of fatigue crack initiation at inclusions. Metall. Trans. A
**1982**, 13, 117–123. [Google Scholar] [CrossRef] - Sinz, U. Schwingfestigkeit von Common-Rail Komponenten unter Berücksichtigung von seltenen nichtmetallischen Einschlüssen. Ph.D. Thesis, Technische Universität Kaiserslautern, Kaiserslautern, Germany, 2017. [Google Scholar]
- Cyril, N.; Fatemi, A.; Cryderman, B. Effects of Sulfur Level and Anisotropy of Sulfide Inclusions on Tensile, Impact, and Fatigue Properties of SAE 4140 Steel. SAE Int. J. Mater. Manuf.
**2009**, 1, 218–227. [Google Scholar] [CrossRef] - Temmel, C.; Ingesten, N.G.; Karlsson, B. Fatigue anisotropy in cross-rolled, hardened medium carbon steel resulting from MnS inclusions. Metall. Mater. Trans. A
**2006**, 37, 2995–3007. [Google Scholar] [CrossRef] - Hosseini, S.B.; Temmel, C.; Karlsson, B.; Ingesten, N.G. An In-Situ Scanning Electron Microscopy Study of the Bonding between MnS Inclusions and the Matrix during Tensile Deformation of Hot-Rolled Steels. Metall. Mater. Trans. A
**2007**, 38, 982–989. [Google Scholar] [CrossRef] - Maciejewski, J. The Effects of Sulfide Inclusions on Mechanical Properties and Failures of Steel Components. J. Fail. Anal. Prev.
**2015**, 15, 169–178. [Google Scholar] [CrossRef] - Åman, M.; Okazaki, S.; Matsunaga, H.; Marquis, G.B.; Remes, H. Interaction effect of adjacent small defects on the fatigue limit of a medium carbon steel. Fatigue Fract. Eng. Mater. Struct.
**2017**, 40, 130–144. [Google Scholar] [CrossRef] - Murakami, Y. Effects of Small Defects and Nonmetallic Inclusions on the Fatigue Strength of Metals. JSME Int. J. Ser. 1 Solid Mech. Strength Mater.
**1989**, 32, 167–180. [Google Scholar] [CrossRef] - Murakami, Y.; Kodama, S.; Konuma, S. Quantitative evaluation of effects of non-metallic inclusions on fatigue strength of high strength steels. I: Basic fatigue mechanism and evaluation of correlation between the fatigue fracture stress and the size and location of non-metallic inclusions. Int. J. Fatigue
**1989**, 11, 291–298. [Google Scholar] [CrossRef] - Zhou, S.; Murakami, Y.; Beretta, S.; Fukushima, Y. Experimental investigation on statistics of extremes for three-dimensional distribution of non-metallic inclusions. Mater. Sci. Technol.
**2002**, 18, 1535–1543. [Google Scholar] [CrossRef] - Manonukul, A.; Dunne, F.P.E. High- and low-cycle fatigue crack initiation using polycrystal plasticity. Proc. R. Soc. London. Ser. A Math. Phys. Eng. Sci.
**2004**, 460, 1881–1903. [Google Scholar] [CrossRef] - McDowell, D.; Dunne, F. Microstructure-sensitive computational modeling of fatigue crack formation. Int. J. Fatigue
**2010**, 32, 1521–1542. [Google Scholar] [CrossRef] - Roters, F.; Eisenlohr, P.; Hantcherli, L.; Tjahjanto, D.; Bieler, T.; Raabe, D. Overview of constitutive laws, kinematics, homogenization and multiscale methods in crystal plasticity finite-element modeling: Theory, experiments, applications. Acta Mater.
**2010**, 58, 1152–1211. [Google Scholar] [CrossRef] - Przybyla, C.; Prasannavenkatesan, R.; Salajegheh, N.; McDowell, D.L. Microstructure-sensitive modeling of high cycle fatigue. Int. J. Fatigue
**2010**, 32, 512–525. [Google Scholar] [CrossRef] - Shenoy, M.; Zhang, J.; McDowell, D. Estimating fatigue sensitivity to polycrystalline Ni-base superalloy microstructures using a computational approach. Fatigue Fract. Eng. Mater. Struct.
**2007**, 30, 889–904. [Google Scholar] [CrossRef] - Cruzado, A.; LLorca, J.; Segurado, J. Modeling cyclic deformation of inconel 718 superalloy by means of crystal plasticity and computational homogenization. Int. J. Solids Struct.
**2017**, 122–123, 148–161. [Google Scholar] [CrossRef] - Briffod, F.; Shiraiwa, T.; Enoki, M. Microstructure modeling and crystal plasticity simulations for the evaluation of fatigue crack initiation in alpha-iron specimen including an elliptic defect. Mater. Sci. Eng. A
**2017**, 695, 165–177. [Google Scholar] [CrossRef] - Boeff, M.; ul Hassan, H.; Hartmaier, A. Micromechanical modeling of fatigue crack initiation in polycrystals. J. Mater. Res.
**2017**, 32, 4375–4386. [Google Scholar] [CrossRef] - Gillner, K.; Münstermann, S. Numerically predicted high cycle fatigue properties through representative volume elements of the microstructure. Int. J. Fatigue
**2017**, 105, 219–234. [Google Scholar] [CrossRef] - Briffod, F.; Shiraiwa, T.; Enoki, M. Modeling and Crystal Plasticity Simulations of Lath Martensitic Steel under Fatigue Loading. Mater. Trans.
**2018**, 60. [Google Scholar] [CrossRef] - Schäfer, B.J.; Sonnweber-Ribic, P.; ul Hassan, H.; Hartmaier, A. Micromechanical Modelling of the Influence of Strain Ratio on Fatigue Crack Initiation in a Martensitic Steel-A Comparison of Different Fatigue Indicator Parameters. Materials
**2019**, 12, 2852. [Google Scholar] [CrossRef] [PubMed] - Brückner-Foit, A.; Huang, X. Numerical simulation of micro-crack initiation of martensitic steel under fatigue loading. Int. J. Fatigue
**2006**, 28, 963–971. [Google Scholar] [CrossRef] - Hallberg, H.; Ås, S.K.; Skallerud, B. Crystal plasticity modeling of microstructure influence on fatigue crack initiation in extruded Al6082-T6 with surface irregularities. Int. J. Fatigue
**2018**, 111, 16–32. [Google Scholar] [CrossRef] - Castelluccio, G.M.; McDowell, D.L. A mesoscale approach for growth of 3D microstructurally small fatigue cracks in polycrystals. Int. J. Damage Mech.
**2014**, 23, 791–818. [Google Scholar] [CrossRef] - Musinski, W.D.; McDowell, D.L. On the eigenstrain application of shot-peened residual stresses within a crystal plasticity framework: Application to Ni-base superalloy specimens. Int. J. Mech. Sci.
**2015**, 100, 195–208. [Google Scholar] [CrossRef] - Gallo, P. On the Crack-Tip Region Stress Field in Molecular Systems: The Case of Ideal Brittle Fracture. Adv. Theory Simul.
**2019**, 2. [Google Scholar] [CrossRef] - Gallo, P.; Hagiwara, Y.; Shimada, T.; Kitamura, T. Strain energy density approach for brittle fracture from nano to macroscale and breakdown of continuum theory. Theor. Appl. Fract. Mech.
**2019**, 103. [Google Scholar] [CrossRef] [Green Version] - Ye, W.; Efthymiadis, P.; Pinna, C.; Ma, A.; Shollock, B.; Dashwood, R. Experimental and modelling study of fatigue crack initiation in an aluminium beam with a hole under 4-point bending. Int. J. Solids Struct.
**2018**, 138, 87–96. [Google Scholar] [CrossRef] - Fan, J.; McDowell, D.L.; Horstemeyer, M.F.; Gall, K. Cyclic plasticity at pores and inclusions in cast Al–Si alloys. Eng. Fract. Mech.
**2003**, 70, 1281–1302. [Google Scholar] [CrossRef] - Gall, K.; Horstemeyer, M.F.; Degner, B.W.; McDowell, D.L.; Fan, J. On the driving force for fatigue crack formation from inclusions and voids in a cast A356 aluminum alloy. Int. J. Fract.
**2001**, 108, 207–233. [Google Scholar] [CrossRef] - Carroll, J.; Brewer, L.; Battaile, C.; Boyce, B.; Emery, J. The effect of grain size on local deformation near a void-like stress concentration. Int. J. Plast.
**2012**, 39, 46–60. [Google Scholar] [CrossRef] - Battaile, C.C.; Emery, J.M.; Brewer, L.N.; Boyce, B.L. Crystal plasticity simulations of microstructure-induced uncertainty in strain concentration near voids in brass. Philos. Mag.
**2015**, 95, 1069–1079. [Google Scholar] [CrossRef] - Gillner, K.; Henrich, M.; Münstermann, S. Numerical study of inclusion parameters and their influence on fatigue lifetime. Int. J. Fatigue
**2018**, 111, 70–80. [Google Scholar] [CrossRef] - Prasannavenkatesan, R.; Przybyla, C.P.; Salajegheh, N.; McDowell, D. Simulated extreme value fatigue sensitivity to inclusions and pores in martensitic gear steels. Eng. Fract. Mech.
**2011**, 78, 1140–1155. [Google Scholar] [CrossRef] - Salajegheh, N. Microstructure-Sensitive Weighted Probability Approach for Modeling Surface to Bulk Transition of High Cycle Fatigue Failures Dominated by Primary Inclusions. Ph.D. Thesis, Georgia Institute of Technology, Atlanta, Georgia, 2011. [Google Scholar]
- Prithivirajan, V.; Sangid, M.D. The role of defects and critical pore size analysis in the fatigue response of additively manufactured IN718 via crystal plasticity. Mater. Des.
**2018**, 150, 139–153. [Google Scholar] [CrossRef] - Bandyopadhyay, R.; Sangid, M.D. Crystal plasticity assessment of inclusion- and matrix-driven competing failure modes in a nickel-base superalloy. Acta Mater.
**2019**, 177, 20–34. [Google Scholar] [CrossRef] - Gu, C.; Lian, J.; Bao, Y.; Münstermann, S. Microstructure-based fatigue modelling with residual stresses: Prediction of the microcrack initiation around inclusions. Mater. Sci. Eng. A
**2019**, 751, 133–141. [Google Scholar] [CrossRef] - Clark, B.; Castelluccio, G.; Reiterer, M.; McDowell, D.; Neu, R. Microstructure-sensitive fatigue modelling of medical-grade fine wire. Fatigue Fract. Eng. Mater. Struct.
**2019**, 42, 152–165. [Google Scholar] [CrossRef] - Zhang, T.; Jiang, J.; Britton, B.; Shollock, B.; Dunne, F. Crack nucleation using combined crystal plasticity modelling, high-resolution digital image correlation and high-resolution electron backscatter diffraction in a superalloy containing non-metallic inclusions under fatigue. Proc. R. Soc. A Math. Phys. Eng. Sci.
**2016**, 472, 20150792. [Google Scholar] [CrossRef] [PubMed] - Naragani, D.; Sangid, M.D.; Shade, P.A.; Schuren, J.C.; Sharma, H.; Park, J.S.; Kenesei, P.; Bernier, J.V.; Turner, T.J.; Parr, I. Investigation of fatigue crack initiation from a non-metallic inclusion via high energy x-ray diffraction microscopy. Acta Mater.
**2017**, 137, 71–84. [Google Scholar] [CrossRef] - Schäfer, B.J.; Song, X.; Sonnweber-Ribic, P.; ul Hassan, H.; Hartmaier, A. Micromechanical Modelling of the Cyclic Deformation Behavior of Martensitic SAE 4150—A Comparison of Different Kinematic Hardening Models. Metals
**2019**, 9, 368. [Google Scholar] [CrossRef] [Green Version] - Kitahara, H.; Ueji, R.; Tsuji, N.; Minamino, Y. Crystallographic features of lath martensite in low-carbon steel. Acta Mater.
**2006**, 54, 1279–1288. [Google Scholar] [CrossRef] - Morito, S.; Tanaka, H.; Konishi, R.; Furuhara, T.; Maki, T. The morphology and crystallography of lath martensite in Fe-C alloys. Acta Mater.
**2003**, 51, 1789–1799. [Google Scholar] [CrossRef] - Cayron, C. ARPGE: A computer program to automatically reconstruct the parent grains from electron backscatter diffraction data. J. Appl. Crystallogr.
**2007**, 40, 1183–1188. [Google Scholar] [CrossRef] [Green Version] - Kitahara, H.; Ueji, R.; Ueda, M.; Tsuji, N.; Minamino, Y. Crystallographic analysis of plate martensite in Fe—28.5 at. % Ni by FE-SEM/EBSD. Mater. Charact.
**2005**, 54, 378–386. [Google Scholar] [CrossRef] - Murakami, Y. Inclusion Rating by Statistics of Extreme Values and Its Application to Fatigue Strength Prediction and Quality Control of Materials. J. Res. Natl. Inst. Stand. Technol.
**1994**, 99, 345–351. [Google Scholar] [CrossRef] - Sandström, R.; Karlsson, L. Transfer of two dimensional inclusion size distribution to three dimensions. In Proceedings of the Swedish Symposium on Non-Metallic Inclusions in Steel, Uddeholm, Sweden, 27–29 April 1981; pp. 242–268. [Google Scholar]
- Anderson, C.; Shi, G.; Atkinson, H.; Sellars, C. The precision of methods using the statistics of extremes for the estimation of the maximum size of inclusions in clean steels. Acta Mater.
**2000**, 48, 4235–4246. [Google Scholar] [CrossRef] - Spriestersbach, D.; Grad, P.; Kerscher, E. Influence of different non-metallic inclusion types on the crack initiation in high-strength steels in the VHCF regime. Int. J. Fatigue
**2014**, 64, 114–120. [Google Scholar] [CrossRef] - Dassault Systèmes. Abaqus Documentation; MIT Press: Cambridge, MA, USA, 2018. [Google Scholar]
- Lu, S.; Pister, K. Decomposition of deformation and representation of the free energy function for isotropic thermoelastic solids. Int. J. Solids Struct.
**1975**, 11, 927–934. [Google Scholar] [CrossRef] - Lee, E.H. Elastic-plastic deformation at finite strains. J. Appl. Mech.
**1969**, 36, 1–6. [Google Scholar] [CrossRef] - Sherby, O.D.; Wadsworth, J.; Lesuer, D.R.; Syn, C.K. Revisiting the Structure of Martensite in Iron-Carbon Steels. Mater. Trans.
**2008**, 49, 2016–2027. [Google Scholar] [CrossRef] [Green Version] - Michiuchi, M.; Nambu, S.; Ishimoto, Y.; Inoue, J.; Koseki, T. Relationship between local deformation behavior and crystallographic features of as-quenched lath martensite during uniaxial tensile deformation. Acta Mater.
**2009**, 57, 5283–5291. [Google Scholar] [CrossRef] - Rice, J. Inelastic constitutive relations for solids: An internal-variable theory and its application to metal plasticity. J. Mech. Phys. Solids
**1971**, 19, 433–455. [Google Scholar] [CrossRef] - Hutchinson, J.W. Bounds and self-consistent estimates for creep of polycrystalline materials. Proc. R. Soc. Lond. A Math. Phys. Eng. Sci.
**1976**, 348, 101–127. [Google Scholar] [CrossRef] - Peirce, D.; Asaro, R.; Needleman, A. Material rate dependence and localized deformation in crystalline solids. Acta Metall.
**1983**, 31, 1951–1976. [Google Scholar] [CrossRef] - Ohno, N.; Wang, J.D. Kinematic hardening rules with critical state of dynamic recovery, part I: Formulation and basic features for ratchetting behavior. Int. J. Plast.
**1993**, 9, 375–390. [Google Scholar] [CrossRef] - Lubarda, V.A. Constitutive theories based on the multiplicative decomposition of deformation gradient: Thermoelasticity, elastoplasticity, and biomechanics. Const. Theor. Based Mult. Decompos. Deform. Gradient Thermoelast. Elastoplast. Biomech.
**2004**, 57, 95–108. [Google Scholar] [CrossRef] - Vujosevic, L.; Lubarda, V.A. Finite-strain thermo elasticity based on multiplicative decomposition of deformation gradient. Theor. Appl. Mech.
**2002**, 28–29, 379–399. [Google Scholar] [CrossRef] - Sweeney, C.; Dunne, F.; McHugh, P.; Leen, S. Micro-scale testing and micromechanical modelling for high cycle fatigue of CoCr stent material. J. Mech. Behav. Biomed. Mater.
**2015**, 46, 244–260. [Google Scholar] [CrossRef] [PubMed] [Green Version] - Fatemi, A.; Socie, D.F. A critical plane approach to multiaxial fatigue damage including ou-of-phase loading. Fatigue Fract. Eng. Mater. Struct.
**1988**, 11, 149165. [Google Scholar] [CrossRef] - Pineau, A.; Forest, S. Effects of inclusions on the very high cycle fatigue behaviour of steels. Fatigue Fract. Eng. Mater. Struct.
**2017**, 40, 1694–1707. [Google Scholar] [CrossRef] - Kitagawa, H.; Takahashi, S. Applicability of fracture mechanics to very small cracks or cracks in the early stage. In Proceedings of the second international conference on mechanical behavior of materials, Boston, MA, USA, 16–20 August 1976; pp. 627–631. [Google Scholar]

**Figure 1.**Martensitic microstructure and corresponding non-metallic inclusions: (

**a**) Schematic visualization of the hierarchical martensitic microstructure, following Kitahara et al. [50]. (

**b**) Inverse pole figure color map with reconstructed prior austenite grain boundaries indicated by white solid lines. (

**c**) Spherical aluminum oxide. (

**d**) Elongated manganese sulfides. The colors in (

**b**) correspond to orientations perpendicular to the observed plane.

**Figure 2.**Statistical evaluation of failure-relevant non-metallic inclusions in SAE 4150: (

**a**) Experimental inclusion data and generalized extreme value distributions for oxidic and sulfidic inclusions with respect to the defect length scale λ. (

**b**) Experimental inclusion data and generalized extreme value distributions for oxidic and sulfidic inclusions with respect to aspect ratio.

**Figure 3.**Finite element model and applied boundary conditions of the reference configuration without defect. Prior austenite grain boundaries are indicated by black solid lines.

**Figure 4.**Schematic visualization of a statistical volume element containing a defect with diameter D exhibiting different possible inclusion–matrix interface configurations. In addition, the two different mesh regions within the SVE are indicated correspondingly.

**Figure 5.**Schematic visualization of the modeling methodology of the manganese sulfides within the martensitic microstructure: (

**a**) Schematic visualization of the martensitic microstructure with the manganese sulfide (Manganese sulfide shown as orange inclusion). (

**b**) Detail of the spatial distribution of tie constraint and contact modeling schemes and (

**c**) detail of the spatial position of the manganese sulfide with respect to loading axis.

**Figure 6.**Schematic representation of the inclusion and defect variants of the micromechanical design of experiment (DOE). Five-level hierarchical structure of the DOE: (1) Inclusion types and interfaces. (2) Inclusion and defect sizes represented by diameters (D) and aspect ratios (AR). (3) Defect geometries expressed by aspect ratios. (4) Microstructural variations ranging from M1–M3 and finally (5) the different applied total strain amplitudes.

**Figure 7.**Effect of local crystallographic variations around voids (AR = 1.0) on fatigue crack initiation behavior for ε

_{a,t}= 0.50%. Radial path plots through the individual hot spot of each SVE. (

**a**) Path plot for void D = 18 μm. (

**b**) Path plot for void D = 36 μm and (

**c**) Path plot for void D = 110 μm. One of the fatigue crack nucleation hot spots of the investigated voids is exemplarily depicted in Figure 10.

**Figure 8.**Residual stress distribution around a perfectly bonded Al

_{2}O

_{3}-inclusions with an aspect ratio of AR = 1. (

**a**) Martensitic microstructure with an embedded inclusion. (

**b**) Radial residual stress distribution. (

**c**) Circumferential residual stress distribution.

**Figure 9.**Residual stresses around oxidic inclusions. (

**a**) Comparison of predicted radial (σ

_{rad}) and circumferential (σ

_{circ}) residual stresses around an inclusion by micromechanical modeling and isotropic material modeling. (

**b**) Effect of superimposed residual stresses on fatigue crack nucleation behavior at different loading levels. The location of one fatigue crack nucleation hot spot of the investigated perfectly bonded inclusions is exemplarily depicted in Figure 10.

**Figure 10.**Contour plots of the von Mises stress in MPa and the dimensionless Fatemi–Socie parameter around the defects with D = 110 μm are shown at the end of fifths fatigue loading cycles in the first and second column, respectively. The bonded inclusion, partly debonded inclusion, cracked inclusion and the void are shown in the first, second, third and fourth row, respectively. The individual fatigue crack nucleation hotspots are indicated with a white arrow in the Fatemi–Socie plot. The contour plot values correspond to the local integration points in the center of each finite element.

**Figure 11.**Comparison of the non-local Fatemi–Socie parameter distribution as a function of the far-field applied total strain amplitude for the different inclusion–matrix interface configurations. (

**a**) Inhomogeneity with diameter D = 18 μm. (

**b**) Inhomogeneity with diameter D = 36 μm. (

**c**) Inhomogeneity with diameter D = 110 μm.

**Figure 12.**Non-local Fatemi–Socie responses of the different inclusion–matrix configurations as a function of the different defect sizes with an aspect ratio of AR = 1.0, for: (

**a**) 0.10% applied total strain amplitude at R

_{ε}= −1 and (

**b**) 0.50% applied total strain amplitude at R

_{ε}= −1. The different colored dashed lines represent the arithmetical average of the three microstructural representatives of each defect type.

**Figure 13.**Schematic visualization of the models to investigate the influence of aspect ratio on fatigue crack initiation. Therefore, voids within the martensitic microstructure are used. These defects exhibit different aspect ratios increasing from left to right from AR = 1.0, 2.0 up to 10.0.

**Figure 14.**Non-local Fatemi–Socie fatigue crack initiation simulation results of voids with a major axis of 110 μm and three different aspect ratios. The aspect ratio is represented as the ratio of the major and minor defect axes. (

**a**) Loading level of ε

_{a,t}= 0.10% and (

**b**) loading level of ε

_{a,t}= 0.50%.

**Figure 15.**Non-local Fatemi–Socie parameter as a function of the manganese sulfide aspect ratio. The colored markers of each aspect ratio represent the different microstructural realizations. The fully reversed strain-controlled loading was perpendicular to the manganese sulfide with: (

**a**) A total strain amplitude of ε

_{a,t}= 0.10% and (

**b**) with a total strain amplitude of ε

_{a,t}= 0.50%.

**Figure 16.**Fatigue crack initiation lifetime results for the martensitic steel with / without varying defects under fully reversed strain-controlled loading. By means of the Fatemi–Socie metric, micromechanical simulations were performed for: (a) Defects with diameters of D = 110 μm. (b) Defects with diameters of D = 36 μm. (c) Defects with diameters of D = 18 μm and (d) for manganese sulfides with varying aspect ratios and orientations to loading axis. Arithmetic average linear fatigue lifetime curves are shown for each defect type in the corresponding color. The abbreviation PD stands for partially debonded and AR for aspect ratio.

Material | C | Si | Mn | P | S | Cr | Mo |
---|---|---|---|---|---|---|---|

SAE 4150 | 0.52 | 0.26 | 0.74 | 0.014 | 0.008 | 1.31 | 0.18 |

**Table 2.**Derived inclusion properties of oxidic and sulfidic non-metallic inclusions in SAE 4150. Extracted defect length scale $\lambda $, corresponding diameter and aspect ratio values belonging to the 10th, 50th and 90th percentile of the underlying generalized extreme value distributions.

Cumulative Probability | Oxidic Non-Metallic Inclusions | Sulfidic Non-Metallic Inclusions | ||||
---|---|---|---|---|---|---|

P = 10% | P = 50% | P = 90% | P = 10% | P = 50% | P = 90% | |

Defect length scale λ in μm | 16 | 32 | 97 | 16 | 43 | 116 |

Diameter in μm | 18 | 36.2 | 110 | - | - | - |

Aspect ratio [-] | 1.2 | 2.2 | 10 | 10 | 25 | 54 |

**Table 3.**Mechanical properties of the considered inclusion types and the steel matrix [3].

Chemical Composition | Young’s Modulus E | Poisson’s Ratio ν | Coefficient of Thermal Expansion ${\mathit{\alpha}}_{\mathit{T}}$ |
---|---|---|---|

Al_{2}O_{3} | 389 GPa | 0.25 | 8.0 × ${10}^{-6}$ 1/K |

MnS | 69 GPa | 0.30 | 18.1 × ${10}^{-6}$ 1/K |

Steel Matrix | - | - | 12.5 × ${10}^{-6}$ 1/K |

**Table 4.**Set of crystal plasticity parameters for SAE 4150 (39 HRC) at room temperature [49].

Elastic Constants | Flow Rule Parameters | Kinematic Hardening Parameters | |||
---|---|---|---|---|---|

${C}_{11}$ | 253.1 GPa | ${\dot{\gamma}}_{0}$ | 0.001 s${}^{-1}$ | A | 65.506 GPa |

${C}_{22}$ | 132.4 GPa | ${\tau}_{c,0}^{\alpha}$ | 209 MPa | B | 499 |

${C}_{44}$ | 75.8 GPa | m | 100 | M | 8 |

**Table 5.**Ratio of the maximum to the minimum non-local Fatemi–Socie response of three considered microstructural realizations.

Strain Amplitude | D = 110 $\mathsf{\mu}$m | D = 36 $\mathsf{\mu}$m | D = 18 $\mathsf{\mu}$m |
---|---|---|---|

0.10% | 2.35 | 5.10 | 1.98 × ${10}^{5}$ |

0.30% | 1.66 | 1.08 | 1.46 |

0.50% | 1.52 | 1.60 | 2.02 |

© 2019 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Schäfer, B.J.; Sonnweber-Ribic, P.; ul Hassan, H.; Hartmaier, A.
Micromechanical Modeling of Fatigue Crack Nucleation around Non-Metallic Inclusions in Martensitic High-Strength Steels. *Metals* **2019**, *9*, 1258.
https://doi.org/10.3390/met9121258

**AMA Style**

Schäfer BJ, Sonnweber-Ribic P, ul Hassan H, Hartmaier A.
Micromechanical Modeling of Fatigue Crack Nucleation around Non-Metallic Inclusions in Martensitic High-Strength Steels. *Metals*. 2019; 9(12):1258.
https://doi.org/10.3390/met9121258

**Chicago/Turabian Style**

Schäfer, Benjamin Josef, Petra Sonnweber-Ribic, Hamad ul Hassan, and Alexander Hartmaier.
2019. "Micromechanical Modeling of Fatigue Crack Nucleation around Non-Metallic Inclusions in Martensitic High-Strength Steels" *Metals* 9, no. 12: 1258.
https://doi.org/10.3390/met9121258